**4. Defect stability – formation energy and concentration 34**

**6.2. Charged defects in bulk MgO**

**6.2.3. Opt-HSE for charge-transition levels and formation energies**

6.2. Charged defects in bulk MgO

6.2. Charged defects in bulk MgO

**Table 6.3.:** G^{bulk,q}_{f} (1/L → 0) and coefficients a^{q}_{1} and a^{q}_{3} as obtained with LDA and PBE
exchange-correlation (xc) functionals forǫ_{F}=VBM andµ_{O}= 1/2E_{O}^{tot}_{2}.

xc functional q G^{bulk,q}_{f} (1/L→0)(eV) a^{q}_{1}(eVÅ) a^{q}_{3}(eVÅ^{3})

LDA 0 8.62 0 0

1 6.03 -2.17 20.94

2 4.21 -8.82 162.49

PBE 0 7.09 0 0

1 4.54 -1.91 20.77

2 2.82 -7.96 167.27

charged F centers in MgO correctly. To address this issue, the dependence of formation energies and of charge-transition levels on the exchange-correlation treatment is further explored.

The charge-transition level (q + 1/q) corresponds to the Fermi level position where point
defects in charge statesq+ 1and qare in thermodynamic equilibrium with each other, so that
their formation energies coincide. The charge-transition level between the singly charged and
the charge-neutral F centers is therefore given by the equilibrium conditionG^{1}_{f} =G^{0}_{f}, which can
be written in terms of total energies and chemical potentials as

E_{vac}^{+} −E_{host}^{+} +µ_{O}+ǫ_{F} =E_{vac}^{0} −E_{host}^{0} +µ_{O}. (6.4)
The charge-transition level follows as

(+/0) =E_{vac}^{0} −E_{host}^{0} − E_{vac}^{+} −E^{+}_{host}

. (6.5)

In analogy, the charge transition level between the doubly charged and the singly charged F centers is

(2 +/+) =E_{vac}^{+} −E_{host}^{+} − E_{vac}^{2+}−E_{host}^{2+}

. (6.6)

When the neutralizing background method is applied for charge compensation, the host system for both defect states are identically given by the neutral, pristine MgO bulk system and the expression reduces to

(+/0) =E_{vac}^{0} −E_{vac}^{+} . (6.7)
In analogy, the charge-transition level between F^{2+}and F^{+}centers can be expressed as

(2 +/+) =E_{vac}^{+} −E_{vac}^{2+}. (6.8)
To see how the charge-transition levels and formation energies depend on (α,ω), the
extrap-olated formation energiesG^{bulk,q}_{f} for F^{0}, F^{+}, and F^{2+} centers in the dilute limit are computed
for varying HSE parameter sets as a function of Fermi energy. The respective charge-transition
levels(2 +/+)and(+/0)can then be obtained at the formation energy intersections, as shown
for the example of HSE06 in Fig.6.13a. Here, oxygen-rich conditions are considered. Changing
the oxygen chemical potential results in a constant shift in formation energies (see Eq.4.1). For

6.2. Charged defects in bulk MgO example, at a chemical potential of -0.5 eV below the oxygen-rich limit, all formation energies in Fig.6.13a are shifted down by -0.5 eV.

Bothp-type MgO, where the Fermi level is close to VBM, andn-type MgO, where the Fermi
level is close to CBm, are covered in Fig. 6.13a. In p-type MgO, q = 2 is the most stable
charge state of the bulk F center. Inn-type MgO, F^{0}is the most stable defect, but its formation
energy is very high. In the following, the focus is onp-type material, because of its intriguing
catalytic properties that have been outlined in the introduction (Sec.1). Only inp-type MgO the
concentration of oxygen vacancies, namely F^{2+} centers, in thermodynamic equilibrium can be
significant.

**Figure 6.13.: a) Formation energies of oxygen vacancies in bulk MgO,**G^{bulk,q}_{f} , in the dilute
limit, calculated with HSE06 using (Eq.4.1) as a function of Fermi energy, in the oxygen-rich
limit. The energy zero ofǫ_{F}is at the VBM. Charge-transition levels (2+/+) and (+/0) are marked
by arrows. b) VBM, CBm, and charge-transition levels (Eq.6.5-6.6) for different functionals of
the HSE family. The energy zero is at the vacuum level.

The fact that, compared to the neutral F center, the formation energies of charged defects
depend much stronger on the exchange-correlation functional, hints at a dependence of the
VBM energy level (the Fermi level in this system) on exchange-correlation treatment, since
only for charged defects the formation energy depends on the Fermi energy (Eq. 4.1, see also
Ref. [205]). To investigate the dependence further, the electronic structure, including VBM,
CBm, and charge-transition levels, is considered for each functional and aligned at the energy
level in vacuum. Setting the energy zero to the vacuum level corresponds to calculating
forma-tion energies and charge-transiforma-tion levels for a situaforma-tion, where the Fermi level is the vacuum
level. This is only considered to gain a better understanding, why for the realistic situation,
whereǫ_{F} = VBM, the formation energies depend on the exchange-correlation functional. The
vacuum level is a well-defined reference energy, which is easily accessible in cluster calculations
and can also be determined for a periodic bulk model by performing a calculation for a periodic
slab of the pristine MgO (100) surface. A vacuum region of≈200Å separates repeating 5-layer
MgO slabs, where the potential in the middle of this vacuum region is the vacuum levelE_{VAC}^{Surf}
for the surface calculation. To obtain the energy difference between VBM and vacuum level

6.2. Charged defects in bulk MgO
for the bulk system VBM^{Bulk}_{VAC}, the difference betweenE_{VAC}^{Surf} and the 1score level of
magne-siumE_{core}^{Surf} in the middle, bulk-like layer of the slab is determined. This difference is added to
the magnesium 1score level in the bulk system E_{core}^{Bulk}, and the resulting bulk vacuum level is
subtracted from the bulk VBME^{Bulk}_{VBM}obtained in the periodic bulk calculation

VBM^{Bulk}_{VAC}=E_{VBM}^{Bulk} −

E_{core}^{Bulk}+ (E_{VAC}^{Surf} −E_{core}^{Surf})

. (6.9)

VBM^{Bulk}_{VAC}is converged with respect to slab separation and slab thickness. The calculated values
forVBM^{Bulk}_{VAC}are−5.7 eVfor PBE,−6.8 eVfor HSE06, and−7.2 eVfor PBE0.

**Table 6.4.:** G^{bulk,q}_{f} , (+/0), and (2+/+) in eV for F^{0}, F^{+}, and F^{2+} centers in MgO bulk in the
dilute limit, calculated with different exchange-correlation functionals using periodic boundary
conditions (pbc), employing FHI-aims. The Fermi level is the vacuum level, the numbers in
parentheses correspond to the Fermi level at VBM, µ_{O} is 1/2E_{O}^{tot}_{2}. HSE06 provides the best
accuracy within the HSE family of functionals for the formation energy of F centers in MgO
(discussed below), and the corresponding numbers are therefore highlighted. The calculations
in Ref. [30] were performed using embedded clusters (ecm).

Method F^{0} F^{+} F^{2+} (+/0) (2+/+)

PBE-pbc 7.09 10.24 (4.54) 14.22 (2.82) -3.15 (2.55) -3.98 (1.72) HSE06-pbc 7.04 10.20 (3.40) 14.16 (0.56) -3.16 (3.64) -3.96 (2.84) PBE0-pbc 7.07 10.15 (2.95) 14.24 (-0.16) -3.08 (4.12) -4.09 (3.11)

HF+MP2-ecm [30] 7.35 9.98 13.88 -2.63 -3.90

VBM, CBm, and charge-transition levels are shown in Fig.6.13b for different functionals of
the HSE family, when the Fermi level is the energy level in vacuum. In agreement with related
work on ZnO and ZrO_{2}*by Ramprasad et al. [186], the charge-transition levels (2+/+) and (+/0)*
for F centers in bulk MgO are almost independent on the exchange-correlation functional within
the HSE family, when the Fermi level is the vacuum level. Indeed, in MgO this is even true
for the corresponding formation energiesG^{bulk,q}_{f} . Bulk F center formation energies and
charge-transition levels forǫ_{F} at the vacuum energy level andǫ_{F} = VBM (in parenthesis), calculated
with different exchange-correlation functionals, are summarized in Table6.4.

Whenǫ_{F}is at the vacuum level, formation energies calculated using periodic boundary
condi-tions and the PBE, HSE06, and PBE0 functionals as representative HSE members, agree within
0.05 eV for F^{0}, 0.09 eV for F^{+}, and 0.08 eV for F^{2+}. The respective deviations for the
charge-transition levels are≤0.13 eV.

For the more relevant case, when ǫ_{F} is at the VBM, the formation energies depend almost
linearly on the exchange parameterα, as shown forω = 0.11 bohr^{−1} and ω = 0.3bohr^{−1} in
Fig.6.14. This is mainly due to a linear dependence of the VBM with respect to vacuum on the
exchange parameter, since the charge-transition levels’ positions depend weakly onαwhenǫ_{F}
is the energy in vacuum. Accordingly, the near-linear dependence of the formation energy onα
is approximately twice as strong for F^{2+}as for F^{+}.

6.2. Charged defects in bulk MgO

**Figure 6.14.: Defect formation energies**G^{bulk,q}_{f} in the dilute limit as a function of HSE exchange
parameter α for two choices of the range-separation parameter. Crosses mark the results for
HSE06. The Fermi level is at the VBM, and the chemical potential of oxygenµO= 1/2EO2.

Next, an optimal DFT exchange-correlation functional to describe the formation energies of
F centers in MgO is identified, according to a condition on DFT ionization energies. The term
*ionization energy originally refers to the energy required to remove an electron from a system*
and put it to the vacuum. This concept is used in a wider sense, referring to ionization energy
as the energy required to remove one electron from the system and put it to the Fermi level.

For an F center in charge stateq, the ionization energy at fixed geometry describes the charging of the defect q → q + 1. The charge transition level (q + 1/q), where the energy zero is at the VBM (compare Fig.6.13) can be interpreted as the adiabatic ionization energy, where geometric relaxation due to the change in charge state is accounted for and the removed electron has been brought to the VBM. Since it is found that atomic relaxation around F centers in MgO is described accurately already by the PBE functional, it remains to find HSE parameters that give correct ionization energies at fixed geometry.

The GW approach allows to accurately calculate single-particle excitation energies, which
includes the ionization potential. In practice, GW ionization energies are usually calculated
as a perturbative correction to the Kohn-Sham levels. To distinguish this approach from the
non-perturbative, fully self-consistentGW, it is usually termedG_{0}W_{0}@XCA, where XCA
de-notes the employed exchange-correlation approximation and is replaced by the name of the
DFT functional used as an input. The following approach is inspired by the Xα concept by
Slater [206,207]: Such parameters of the HSE functional are found that the∆SCF ionization
energy, calculated with the corresponding functional opt-HSE, coincides with theG_{0}W_{0}
@opt-HSE ionization energies.

The ionization potential at a fixed defect geometry for a given functional HSE(α,ω) is
I_{∆SCF}^{q→q+1} =E_{vac}^{q+1}+ǫ_{F}−E_{vac}^{q} , (6.10)
where bothEvac^{q} andEvac^{q+1}are extrapolated to the dilute limit. Forǫ_{F} =VBM,I_{∆SCF}^{q→q+1}depends

6.2. Charged defects in bulk MgO on (α, ω). The requirement thatGW and HSE ionization energies agree defines the opt-HSE functional that correctly describes the charge excitation of the defect

I_{G}^{q→q+1}_{0}_{W}_{0} =ǫ_{F}−ǫ^{G}_{HOMO}^{0}^{W}^{0} =^{!} I∆SCF,opt−HSE^{q→q+1} . (6.11)
Here the HOMO level is calculated byG_{0}W_{0}@opt-HSE. An embedded cluster model can be
used to efficiently perform this validation step. The ionization energies I^{0→+} and I^{+→2+} for
ω = 0.11 bohr^{−1} as a function ofα are calculated forǫ_{F} at VBM at F^{0} geometry for the
em-bedded Mg_{6}O_{9} cluster model (Fig. 6.7) using FHI-aims. The Fermi level ǫ_{F} is obtained as
VBM = E_{host}^{+1} −E_{host} using HSE functionals, and from the HOMO of the host system in the
corresponding G_{0}W_{0}@HSE calculations. The ionization potentials show a near-linear
depen-dence on the exchange parameterαfor both∆SCF andG0W0methods (Fig.6.15). The starting
point dependence of theG_{0}W_{0} ionization energies is weak for this system. The intersection
of the linear fits are atα=0.27 for I^{0→+} and α=0.26 for I^{+→2+}, very close toα in HSE06
(α=0.25). The same result is obtained, when the HSE ionization energies are determined from
the highest occupied Kohn-Sham level at half occupation [45,47]. Therefore, HSE06 is used as
an opt-HSE functional that correctly describes the charge excitation of the defect. The difference
in formation energies withα=0.25 instead ofα=0.27 is negligible for F^{0}, less than 0.1 eV for
F^{+}, and less than 0.2 eV for F^{2+}.

**Figure 6.15.: Ionization potentials**I^{q→q+1}at F^{0} geometry calculated for an Mg6O9 embedded
cluster using the∆SCF method with HSE functionals (black circles) and from the HOMO of a
G_{0}W_{0}@HSE calculation (blue squares). The screening parameter is ω = 0.11bohr^{−1}. Solid
and dashed lines show linear fits toI^{0→+} andI^{+→2+} as a function of exchange parameterα.

Red crosses show the Kohn-Sham eigenvalues at half occupation.

Furthermore, it has been found in Sec.6.1that DFT+∆CCSD(T) results of the F^{0}formation
energy are in good agreement with the HSE06 F^{0} formation energy. Thus, HSE06 is the
opt-HSE functional in accordance withGW as well as coupled-cluster results, and can be used to
accurately calculate F^{0}, F^{+}, and F^{2+}center formation energies and related properties in MgO.

6.2. Charged defects in bulk MgO